Unit 4, West Court, Buntsford Park Road, B60 3DX Email: email@example.com Website: ngenco.com Ngenco Clear Paint Protection Spray Stone Chip Resistant Test ASTM D3170, SAE J400 Standard TheWhateverRoadThrowsAtYou.
5 March 2020 5 March 2020 Exposure ExposureCompletionDate:Date:Duration: 1 cycle per specimen Chip Resistance TestExposure Type: ApprovedBy: By: Test Equipment Used: Axel LaboratoryThomasLaboratoryKoerperManagerAllieManager (USA) Q-Lab Deutschland GmbH In den Hallen 30 66115 Saarbrücken 5 March 2020 TESTLaboratoryCERTIFICATETesting NBU-0003Test Address:Company:Number: Unit 4, West Court Buntsford Park Road UNITED KINGDOM. TestNo.Attention:ofSpecimens:Method: SAE J400:2002, Meth. C BlackSpecimen Identification: NGENCO Ltd. Payment Reference: NoneDeviations: Coated metal panels2 Bromsgrove, B60 3DX 1 pint road gravel, 483 kPa, 90° Orientation, 7-10 Seconds at ambient temp Multi-Test Gravelometer (MTG) e o LW0260220
QT PaymentNo: Ref: Specimen Condition: No Exception Test Description: 5 March 2020Date Exposed: Customer No: Test No: NBU-0003 All specimens were received in good condition except: G01175 Chip Resistance TestType of Test: Specimen Description: 2 Coated metal panels 10 cm x 15 cm Black ; Silver 5 March 2020 Irradiance: N/ATestCycle:Method: SAE J400:2002, Meth. C Device Used:Multi-Test Gravelometer (MTG) Filters: 1N/Apint gravel, 483 kPa, 90° orientation, 7-10 seconds
Temperatures: Ambient Humidities: N/A Water type: N/A Relocation: As required Total duration: 1 cycle per specimen LW0260220 Light Source: N/A Deviation: No Evaluations and Reports: Evaluations required. The level of stone chip and road rash protection offered by Ngenco PPS when applied to the original Automotive OEM Clear-Coated paintwork. Impact: QGR Gravelometer Chipping Your Ref: NGENCO Ltd. Unit 4, West Court Buntsford Park Road B60 3DX BROMSGROVE , UNITED KINGDOM Ngenco R&D Department Technical@ngenco.comEmail: Please use the test number above to identify this test in all correspondence. Thank you, Axel AcceleratedKoerperLab
ManagerUpon CompletionReturn Schedule: Special Instructions: StandardReport Type:
Q-Lab Deutschland GmbH To our Client: Your test specimens have been received by us and stone chip resistance testing commenced according to the following:
Failureis determined by the appearance of stone chip damage to the OEM Clear-Coat and Painted Panel No stone stone chip damage to the OEM Clear-Coat denotes aPass
The appearance of the tested sample is then compared to a standard OEM painted and Clear-Coated Panel by way of visual examination.
The NGENCO PPS coated OEM Clear-Coated Paint should show no stone chips in OEM Clear-Coated Paint when removed following the test. (Dents may be present due to the force of impact)
Scope: This Gravelometer test was carried out to evaluate the the level of stone chip / road rash protection offered by NGENCO PPS when applied to the original Automotive OEM Clear-Coated paintwork dr ve der r a everyday dr v d
Specimen size: A 10cm by 15cm panel OEM painted and clear-coated metal panel coated with 200 microns of Ngenco Paint Protection Spray, (PPS). Unit 4, West Court, Buntsford Park Road, B60 3DX Tel: +44 (0) 1527 868275 Email: firstname.lastname@example.org Website: ngenco.com
1.De-Lamination of the Paint Protection from the OEM Clear Coated Panel 2. Checking for evidence of stone chip damage to the OEM Clear-Coated Panel
Followed by the removal of Ngenco PPS to
TestProcedure: An Automotive OEM Clear-Coated and Painted Panel is coated with the recommended film thickness of NGENCO PPS, usually 200 microns. The test sample is mounted in the back of the Gravelometer, and air pressure is used to project gravel at the Oncesample.thetest is complete the sample is then removed and gently wiped off with a clean cloth to check for
Additionally, Q-Lab gravel meets the requirements JIS A 5001 #6 and #7 gravel. Even though this standard has nothing to do with Gravelometer testing, some Japanese automotive OEMs have test methods that refer to it. Q-Lab's gravel is screened to meet the requirements of JIA A5001 #6 and #7.
Data:Thegravel for this test shall be water-worn road gravel, not crushed limestone or rock. The gravel will pass through 15.86 mm (5/8 in) space screen when graded, but be retained on 9.53 mm (3/8 in) space screen. The standard requires that the gravel be screened between screen sizes of 3/8" and 5/8" (9.5 - 15.9 mm). Individual stones from natural gravel are oblong, and thus some of them will pass through one of the screens if oriented in one direction but not fit through the screen if oriented in another direction. What the standard actually means is that the largest stones will have at least one dimension 5/8" and that the smallest stones will have at least one dimension 3/8".
Worn River Gravel (G-699): 9.5 to 15.9 mm (3/8 to 5/8 in), Standard Michigan; used in SAE J400 and ASTM D-3170 Unit 4, West Court, Buntsford Park Road, B60 3DX Email: email@example.com Website: ngenco.com
Result: Pass, No Evidence of Stone Chip Damage in The Original OEM Clear Coat (Dents May Be Present Due to The Force of Impact)
Email: firstname.lastname@example.org Website: ngenco.com st Court, Buntsford Park Road, B60 3DX
Unit 4, West Court, Buntsford Park Road, B60 3DX